Poly(methyl methacrylate)-Supported Polydiacetylene Films: UniqueChromatic Transitions and Molecular SensingKaviya Parambath Kootery, Hao Jiang, Sofiya Kolusheva, T. P. Vinod, Margarita Ritenberg,
Leila Zeiri, Roman Volinsky, Danilo Malferrari, Paola Galletti,, Emilio Tagliavini,,
and Raz Jelinek*,,
Department of Chemistry and Ilse Katz Institute for Nanoscale Science and Technology, Ben-Gurion University of the Negev, BeerSheva 84105, IsraelDepartment of Biomedical Engineering and Computational Science, Aalto University, Helsinki, FinlandInterdipartimental Center for Industrial research (CIRI) Energy & Environment, University of Bologna, via S. Alberto 163, 48123Ravenna, ItalyDepartment of Chemistry G. Ciamician, University of Bologna, via Selmi 2, 40126 Bologna, Italy
ABSTRACT: Polydiacetylenes (PDAs) constitute a family ofconjugated polymers exhibiting unique colorimetric and fluorescencetransitions, and have attracted significant interest as chemo- andbiosensing materials. We spin-coated PDA films upon poly(methylmethacrylate) (PMMA), and investigated the photophysical propertiesand sensing applications of the new PDA configuration. Specifically,the as-polymerized blue PDA layer underwent distinct transformationsto purple, red, and yellow phases, which could be quantified throughconventional color scanning combined with application of imageanalysis algorithms. Furthermore, we recorded a reversible red-purplePDA transition that was induced by ultraviolet irradiation, aphenomenon that had not been reported previously in PDA film systems. We show that distinct color and fluorescencetransitions were induced in the PMMA-supported PDA films by amphiphilic substancessurfactants and ionic liquidsand thatthe chromatic transformations were correlated to the analyte structures and properties. Overall, this study presents a newchromatic PDA film system in which noncovalent interactions between the PMMA substrate and spin-coated PDA give rise todistinct chromatic properties and molecular sensing capabilities.
KEYWORDS: polydiacetylene, colorimetric sensors, spin coating, PMMA, thin films
INTRODUCTIONPolydiacetylenes (PDAs) are -conjugated polymers displayingunique structural and chromatic properties.18 These polymers,first synthesized in the late 1960s, have attracted considerableinterest both scientifically and as promising sensing platforms,primarily because of their visible color transformations(generally from blue to red), induced by varied externalstimuli, such as heat,9 ionic strength,10 mechanical pressures,and interactions with biological and chemical molecules.11,12
Modulation of the fluorescence emission of PDA systems whichusually accompany the color changes has also contributed toprogress in this field as the fluorescence phenomena openedroutes for high sensitivity sensing and microscopic imaging.13,14
The intriguing chromatic properties of PDA assemblies arebelieved to arise from the ene-yne topotactic polymerizationprocess, made possible through self-assembly of the diacetylenemonomers stabilized through a hydrogen bond network.15 Thisgeneric structural/chromatic feature of PDA systems has beenattained in numerous morphologies, including vesicles,16,17 thinfilms,18 fibers,19 stacked domains,20 and others. Notably, recentstudies have shown that color reversibility (generally from the
red phase back to the initial blue phase) could be accomplishedthrough modification of the PDA headgroup moieties.21
Further expanding the technological and scientific scope ofthe field has been the demonstration of PDA assembliesexhibiting colors other than blue and red, including yellow andorange PDA.2224
Supported PDA films, in particular, exhibit distinct practicaladvantages and have attracted considerable interest andresearch activities.25,26 Such assemblies are generally robustand stable, and their molecular and macroscopic properties canbe better controlled than vesicular systems. Film properties canbe also thoroughly analyzed through application of advancedsurface characterization techniques.26 Solid-supported PDAfilms have been constructed via diverse techniques, includingLangmuir monolayers,27 dip-coating,28 and spin-coating.29
Here, we present a study of new PDA films prepared throughspin-coating of the diacetylene monomers onto poly(methyl
Received: March 11, 2014Accepted: May 9, 2014
XXXX American Chemical Society A dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXX
methacrylate) (PMMA), a transparent polymer that is widelyused in many applications, particularly as a glass substitute.30
We found that the PMMA substrate intimately affects thedeposited PDA films and endows interesting chromaticproperties to the system, including chromatic reversibilityinduced by ultraviolet (UV) irradiation, and purple/red/orange/yellow color transformations affected by interactionswith amphiphilic analytes. Specifically, we have testedsurfactants classified as cationic, anionic, and nonionicamphiphiles and ionic liquids (ILs) that exhibit surface-activeproperties because of their structural features.31
EXPERIMENTAL SECTIONMaterials. The diacetylene monomer 10,12-tricosadiynoic acid
(TRCDA) and 1-hexadecyltrimethylammonium bromide (CTAB)were purchased from Alfa Aesar; poly(methyl methacrylate) (PMMA,or Perspex) was purchased from Segalovitch Israel; Tetrahydrofuran(THF) and diethyl ether were purchased from Bio-Lab Ltd;Dichloromethane (DCM), ammonium hydroxide, chloroform(CHCl3) and methanol were purchased from Frutarom Ltd; 2,2,2-Trifluoroethanol, Triton X-100, cetylpyridinium chloride (CPC),oxalyl chloride, dodecylamine, 1-chlorohexadecane, 1-chlorododecane,1-methylimidazole, itaconic acid, 1,6-anhydroglucopyranose (Levoglu-cosan), lauric acid, Pseudomonas cepacia (PS C, lipase immobilized onceramic particles), acetonitrile, activated charcoal (decolorizing),lithium aluminum hydride (LiAlH4), sodium dodecyl sulfate (SDS),and sodium dodecylbenzenesulfonate (SDBS) were purchased fromSigma-Aldrich. All the reagents and solvents were used as receivedwithout further purification.Synthesis. 10,12-Tricosadiyn Amine. Synthesis of 10,12-tricosa-
diyn amine was carried out through a two-step pathway:
(i) TRCDA (570 mg) was dissolved in DCM (20 mL); 2 mL ofoxalyl chloride is added two the solution under an argonatmosphere. Several drops of DMF were then added as catalyst.
The mixture is stirred at room temperature for overnight. Afterthis, the solvent was evaporated and the residue was dissolvedin dry THF (20 mL). The solution was then slowly added to 30mL of ammonium hydroxide (25 %) in an ice bath and stirredovernight. The solvent was evaporated and the residue wasextracted with DCM three times. The organic layer was driedover MgSO4, filtered, and evaporated to dryness.
(ii) The residue obtained in the first step was added to 30 mL ofdiethyl ether. LiAlH4 (550 mg) was added to it while keepingthe solution in an ice bath (Caution! Do not drop LiAlH4powder into ice, which causes a violent reaction). The solution wasstirred overnight and then poured into a saturated solution ofNH4Cl. The aqueous layer was then extracted with ethylacetate. The combined organic layer was washed with saturatedNaCl solution and then dried with MgSO4, filtered andevaporated. The residue was purified with column chromatog-raphy over silica gel. CHCl3:methanol (9:1) was initially usedas solvent, followed by a mixture of 2.5 % NH4OH in methanoland CHCl3.
Ionic Liquids (ILs). 3, 1-dodecyl-3-methylimidazolium chloride,C12mimCl; and 4, 1-hexadecyl-3-methylimidazolium chloride,C16mimCl (the numbers refer to the compounds outlined in Scheme1, below): ILs 3 and 4 were synthesized according to the procedurereported in the literature32 by mixing 1-methylimidazole (1 equiv.)with the corresponding chloroalkane (C12 or C16, 1.1 equiv.) at 50C. After 24 h, the ILs were washed with diethyl ether (2) and ethylacetate (2) to remove unreacted reagents. After solvent separationthe solvent residue was evaporated under reduced pressure. ILssynthesized were dissolved in a small volume of acetonitrile and passedthrough a thin column of activated charcoal and silica gel to excludethe presence of colored impurities often present in ILs.33,34
6:1-lauryl-4-carboxy-2-pyrrolidone, ITAC12 was synthesized undersolventless conditions through adapting a published procedure.35
Briefly, dodecylamine (1 equiv) was added to a two-necked round-bottom flask and heated at 40 C for few minutes until complete
Scheme 1. Structures of the Amphiphilic Compounds Tested: 1, CTAB; 2, CPC; 3, C12mimCl; 4, C16mimCl; 5, C12NH2; 6,ITAC12; 7, C12LG; 8, Triton X-100; 9, SDS; 10, SDBS
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXXB
melting. Itaconic acid (1 equiv) was added to dodecylamine and themixture heated at 100 C for 3 h. The reaction was monitored by thinlayer chromatography (TLC) (cyclohexane:ethyl acetate = 2:8). Theproduct was purified using column chromatography (cyclohexane/ethyl acetate, gradient elution).7:4-O-Lauryl-levoglucosan, C12LG was synthesized and purified
from levoglucosan and lauric acid by Lipase catalyzed esterificationfollowing published procedure.36
Film Preparation. The diacetylene monomers (10,12-tricosadiy-noic acid and 10,12-tricosadiyn amine) were dissolved in a solventcomprising THF and DCM at a 1:1 ratio in a concentration of 45 mg/mL. The solution was filtered through a membrane filter (Millex,Nylon, 0.45 m). The PMMA substrates were cut into circular platesof 1 cm diameter. Forty microliters of the monomer was dropped ontothe PMMA and after 30 s was spin-coated at 2500 rpm for 30 s using aWS-650 LITE spin coater from Laurell Technologies Corporation,USA.In the case of the diacetylene mixture, 10,12-tricosadiyn amine was
mixed with 10,12-tricosadiynoic acid at a weight ratio of 1:9 and therest of the procedure was similar to the above procedure for pure10,12-tricosadiynoic acid. The spin-coated films were irradiated withultraviolet light (254 nm) for 0.5 min to produce the polymerized,blue phase of polydiacetylene.Surfactant-Induced Color Change. The tested amphiphilic
compounds were first dissolved in the solvent 2,2,2-trifluoroethanoland the solution was diluted to a final concentration of 1 mM bymixing with Trizmabase buffer at pH 8. Polymerized PMMA-coatedPDA films were placed in 48-well plates. Three hundred microliters ofsurfactant solutions (1 mM) was added on top of the PDAPMMAfilms and the chromatic changes were recorded.Quantitative Color Analysis. Quantification of the color
transitions was based upon a published procedure for RGB analysisof PDA films.37 Briefly, 48-well plates containing the spin-coated
PMMA-supported PDA films incubated with the amphiphiliccompounds were scanned in the transmitted mode on an Epson4990 Photo scanner to produce 2400 dpi, 24 bit color depth red-green-blue (RGB) images. Digital colorimetric analysis (DCA) wascarried out by extracting RGB channel values for each pixel within thesample spots in the scanned images, and the color change values werecalculated using Matlab R2010 scientific software (The Mathworks,Inc., MA, USA) as detailed previously.37 No major changes were madeto the program, which allowed us to calculate color change from theblue to yellow phases.
DCA utilizes the standard red-green-blue (sRGB) modeltranslating color signals into three distinct values corresponding tothe intensities of red (R), green (G), and blue (B) color channels.Accordingly, the relative intensity of a particular RGB component in ascanned image can be defined as the chromaticity level. For example,the yellow chromaticity level (y) in each pixel was calculated as
= + + +y R G R G B( )/( )
where R (red), G (green), and B (blue) are the three primary colorcomponents. For a defined surface area within a PDA-based sensorwell we classified a quantitative parameter denoted yellow chromaticityshift (YCS) that represents the blue-red and blue-red-yellowtransformations of the pixels in the analyzed film area
= y y y yYCS ( )/( )100%sample 0 max 0
where ysample is the average yellow chromaticity level of all pixels in thescanned surface, y0 is the average yellow level calculated in a blanksurface (blue PDA film) and ymax is the average yellow chromaticitylevel of the maximal blue-yellow transition occurring at the PDA film.In essence, YCS is the normalized change in the chromaticity levelwithin the sensor well surface on which the tested sample wasdeposited.
Figure 1. Experimental scheme and film appearance. (A) Experiment summary: monomer solutions (either pure 10,12-tricosadiynoic acid or 10,12-tricosadiynoic acid/10,12-tricosadiyn amine mixture) were spin-coated upon the PMMA substrate and subsequently polymerized by UV irradiation(254 nm). The different color transformations discussed in the text are shown. (B) Scanning electron microscopy (SEM) image of the PMMAsubstrate used prior to spin-coating. (C) SEM image of the PDA film spin-coated over PMMA.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXXC
UVVis Spectroscopy. UVvis spectroscopy measurements werecarried out at 23 C on a Varioskan (Thermo, Finland).Fluorescence Spectroscopy. Forty-eight-well plates containing
the PMMA-coated PDA films were placed in a multiwall fluorescenceplate reader (Varioskan, Thermo, Finland) at 23 C. All measurementswere carried out using 482 nm excitation. The curves obtained weresmoothed by using a 10 point adjacent averaging.Raman Scattering. Raman spectra were recorded with a Jobin-
Yvon LabRam HR 800 micri-Raman system, equipped with a liquid-N2-cooled detector. The excitation source was an Argon laser (514nm), with a power of 5 mW on the sample. In order to protect thesamples the laser power was reduced by 1000 using ND filters. Thelaser was focused with 100 long-focal-length objective to a spot ofabout 4 m. Measurements were taken with the 600 g mm1 gratingand a confocal microscope with a 100 m hole with a typical exposuretime of 1 min.Scanning Electron Microscopy (SEM). Scanning electron
microscopy (SEM) images were recorded on a JEOL JSM-7400F(Tokyo, Japan) Scanning Electron Microscope. Images were takenafter sputtering a thin film of Au (15 nm thickness) over thesubstrates for better contrast and minimum charging.
RESULTS AND DISCUSSIONFigure 1 depicts the experimental scheme and the filmmorphology. Two diacetylene monomers were employed:10,12-tricosadiynoic acid displaying a carboxylic moiety, and10,12-tricosadiyn amine in which the carboxylic residue wassubstituted with an amine. The monomers, dissolved in a THF/DCM mixture (1:1), were deposited through spin-coating uponcircular-shaped PMMA substrates. Following drying andultraviolet irradiation (254 nm), the PDA/PMMA films(produced by using only 10,12-tricosadiynoic acid), as well asPDA-NH2/PDA/PMMA (produced by using 1:9 mol ratiomixture of 10,12-tricosadiyn amine and 10,12-tricosadiynoicacid) turned intense blue due to the conjugated -system of theplanar polydiacetylene network.1 As outlined in Figure 1A, theblue PDA/PMMA films underwent further colorimetrictransformations into purple, red, or yellow, induced by externalstimuli, discussed in detail below. Images B and C in Figure 1present SEM images of the PMMA surface before and after spincoating, respectively. The initial PMMA surface was flat anduniform (Figure 1B). Spin-coating of PMMA with diacetyleneand subsequent polymerization resulted in appearance ofirregularly-shaped rectangular PDA domains previously de-tected in varied film and vesicle configurations38 (Figure 1C).Figure 2 highlights the colorimetric transformations of
PMMA-supported PDA films induced by heating andsubsequent UV irradiation (similar results were recorded incase of spin coating of the PDA-NH2/PDA mixture, data notshown). Following heating (5 min at 80 C), the PDA/PMMAfilms underwent the well-known blue-red transformation9
(Figure 2A). Intriguingly, however, the red film becamegradually purple upon subsequent irradiation with UV light(254 nm for 30 s, Figure 2A). It should be noted that longerirradiation times of the red PDA/PMMA films did not producea complete back-transformation to blue color. Furthermore, thered-purple transformation was not affected by the extent ofinitial irradiation timesimilar colorimetric results wererecorded even when significantly longer initial irradiation wascarried out (up to 10 min), making sure that complete PDApolymerization was achieved.Spectroscopic analyses in Figure 2B-D indicate that the
purple appearance corresponds to a back-transformation of thePDA film into a blue polymer phase. The UV-vis spectra inFigure 2B confirm that UV irradiation resulted in re-emergence
of the peak at around 650 nm corresponding to the blue PDAphase. Similarly, the fluorescence emission data in Figure 2Creveal a dramatic attenuation of the PDA fluorescence of thered sample following uv irradiation, corroborating thehypothesis that the UV-induced purple phase of the PDA/PMMA film corresponds to a unique red-blue transformation ofPDA. The Raman scattering data in Figure 2D lend support tothis interpretation, clearly showing that UV irradiation of thered PDA/PMMA films resulted in re-emergence of theprominent peaks at 1450 and 2090 cm1 associated with theblue PDA phase.39 Importantly, the red-purple transition wasreversible, and the red phase of the film re-appeared afterheating. It should be noted that while several studies hadreported temperature-cycled reversible blue-red transforma-tions of PDA systems,40,41 the UV-induced reversible red-bluetransition highlighted in Figure 2 has not been previouslyreported in the literature for PDA films. This phenomenon iseven more remarkable in light of the well-known effect of UVirradiation as an accelerant of blue-red transitions in PDAvesicles and films.39
The chromatic transformations of PDA systems have beenwidely exploited towards development of biological andchemical sensing applications.12,42,43 Accordingly, we inves-tigated the chromatic response of the new PMMA-supportedPDA films upon addition of different analytes (Figures 35).The PDA/PMMA film assemblies are particularly attractive as asensing platform since they are physically robust and stable,exhibit color durability for long time periods (months) and areamenable for mass production. Scheme 1 presents thestructures of representative amphiphilic molecules tested inthis study. Specifically, we examined amphiphilic compounds(compounds 110, Scheme 1) belonging to different classes,
Figure 2. Chromatic transformations induced by heat and ultravioletirradiation. (A) Scanned images of PMMA-supported PDA filmsundergoing heat-induced blue-red transition and subsequent red-purple transformation induced by UV irradiation; (B) UVvisabsorption spectra of the PMMA-supported PDA films shown in A;(C) fluorescence emission spectra of the PMMA-supported PDA filmsshown in A; (D) Raman spectra of the PMMA-supported PDA filmsshown in A.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXXD
including cationic surfactants [1-hexadecyltrimethylammoniumbromide (CTAB) 1, and cetylpyridinium chloride (CPC) 2],ionic liquids (ILs) [1-dodecyl-3-methylimidazolium chloride(C12mimCl) 3, and 1-hexadecyl-3-methylimidazolium chloride(C16mimCl) 4], weak acid/base surfactants [dodecylamine, 5,1-lauryl-4-carboxy-2-pyrrolidone (ITAC12) 6], non-ionic sur-factants [4-O-lauryl-1,6-anhydroglucopyranose (C12LG) 7, andTriton X-100 8], and anionic surfactants [sodium dodecylsulfate (SDS) 9 and sodium dodecylbenzenesulfonate (SDBS)10].Our choice of analytes was aimed to test a broad range of
reagents and environmentally-sensitive solutes exhibiting differ-ent structures, charge, and functional units. Specifically, weexamined nitrogen-, oxygen-, and sulphur- containing mole-cules having the same chain lengths (12 carbon atoms forcompounds 3, 5, 6, 7, 9 and 10 and 16 carbon atoms forcompounds 1, 2, and 4) but displaying different charges (or nocharges) in the polar head. Compounds 5, 6, and 7 can beconsidered as representative renewable surfactants, synthesizedfrom renewable resources.44 Specifically, primary amines suchas compound 5 are produced in industrial processes from lauricacid;45 6 is obtained from the reaction of itaconic acid anddodecylamine 5. Itaconic acid is industrially obtained with highyields in biotechnical processes using substrates like sucrose,glucose, starch hydrolysates, or purified molasses and fungi ofthe genus Aspergillus.46 7 is obtained through enzyme acylationof levoglucosan, a common anhydro-sugar, produced in highyields from the pyrolytic treatment of cellulose.47
Figure 3 presents scanned images of the color trans-formations induced by the analytes upon incubation withPDA/PMMA and PDA-NH2/PDA/PMMA. The choice of thetwo specific sensor compositions was aimed at assessing theeffect of varying the PDA headgroup upon the chromaticproperties and transformations. The images in Figure 3 clearlyshow that the surfactants induced distinct color changes uponincubation with the films. Furthermore, differences in colortransitions are also apparent between films containing the twoPDA derivatives.Specifically, CTAB (1) induced a striking blue-yellow
transformation upon incubation with the PDA/PMMA film,and yellow-orange color in the case of PDA-NH2/PDA/PMMA. In comparison, CPC (2) and the ILs displayingpositively charged bulky headgroups 3 and 4 gave rise toorange-red colors when added to PDA/PMMA, and orange-purple shades upon addition to PDA-NH2/PDA/PMMA. Itappears that the difference in the length of the alkyl chains ofILs 3 and 4 (four carbon atoms) did not play a role in inducing
color changes. Although the ionic compounds 14 and theamine 5, which also is partially protonated in the experimentalconditions, induced significant color changes, as shown inFigure 3, the carboxylate-type surfactant 6, the nonionicsurfactants 7 and 8, and anionic surfactants 9 and 10 producedsmall or insignificant color changes in the PDA/PMMA systemand blue-purple transitions upon incubation with the PDA-NH2/PDA/PMMA films (in case of the nonionic surfactants,Figure 3).The color changes of the PDA/PMMA films can be
quantified through application of a simple image analysisalgorithm,37 providing the means for both comparing thedifferent colors induced, as well as evaluating the time-dependent colorimetric transformations (Figure 4). The kineticcurves in Figure 4 represent the extent of color transformationsthrough combining image analysis of scanned images such asshown in Figure 3 with summation of the red-blue-greencomponents in each pixel.37 Essentially, the %RGB scale
Figure 3. Color transitions induced by the amphiphilic analytes. Scanned images of PDA/PMMA (top row), and PDA-NH2/PDA/PMMA (bottomrow), after addition of the surfactants (concentrations 1 mM). Images were recorded after 40 min incubation.
Figure 4. Quantitative kinetic color curves. Time-dependent %RGBcurves reflecting the extent of blue-red-yellow transformation of the(A) PDA/PMMA film and (B) PDA-NH2/PDA/PMMA film afteraddition of compounds 110.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXXE
measures the blue-red-yellow transformations, in which highvalues correspond to the appearance of a yellow color, whereaslower %RGB reflects less pronounced color transitions (e.g.,blue-purple and blue-red).The %RGB analysis in Figure 4 underscores the significantly
different color transformations both recorded among thecompounds tested, and also between the two PDA filmcompositions. Specifically, high %RGB values were recordedwhen the cationic surfactants (1 and 2) or ILs (3 and 4) wereadded. These compounds furthermore induced almostinstantaneous colorimetric transformations (Figure 4). Thenonionic surfactants (7 and 8), on the other hand, gave rise tomuch lower %RGB values which gradually increased over time.This result likely reflects slow adsorption of these surfactantsonto the PDA films. Note, however, that the %RGB graphs inFigure 4 clearly show that the non-ionic surfactants gave rise togreater color transformations upon addition to the PDA-NH2/PDA/PMMA films, reflecting the enhanced adsorption to thepolar amine moieties. Figure 4 also demonstrates that theanionic surfactants 9 and 10 induced negligible color changesthat are ascribed to electrostatic repulsion to the PDA units thatexhibit residual negative charge. A similar result was recorded in
case of 6, which is anionic at the pH condition employed in theexperiments (pH 8).Interestingly, the %RGB curve recorded for dodecylamine
(5) appears different than the other surfactants tested, initiallyinducing low %RGB values while rapidly increasing after a fewminutes. This distinct kinetic behavior is probably related to themuch smaller headgroup of 5 as compared to the othersurfactants examined, and/or to the presence of the basicnitrogen. Importantly, the quantitative kinetic analysis in Figure4 underscores the differences between the chromatic responsesof PDA/PMMA and PDA-NH2/PMMA: the ionic compoundsinduced higher %RGB when incubated with the (negatively-charged) carboxyl-displaying film, whereas the nonionicsurfactants generally gave rise to steeper %RGB kinetic curvesin case of PDA-NH2/PDA/PMMA.To shed light upon the colorimetric transitions induced by
the surfactants in the PDA/PMMA films we carried outspectroscopic analyses (Figure 5). Specifically, we recordedUVvis spectra and fluorescence emission of representativefilms, together providing insight into the photophysicalproperties of the distinct PDA phases formed. The UVvisspectra in panels A and B in Figure 5 reveal that the yellowPDA phase (induced by incubation of the PDA/PMMA or
Figure 5. Spectroscopic characterization of PMMA-supported PDA films undergoing distinct color transitions. The four compounds shownrepresent different color transitions: CTAB (yellow); C12mimCl (red); triton X-100 (purple); SDBS (magenta). (A) UVvis absorbance spectra ofPDA/PMMA; (B) UVvis absorbance spectra of PDA-NH2/PDA/PMMA; (C) fluorescence emission spectra of PDA/PMMA, excitation 482 nm;(D) fluorescence emission spectra of PDA-NH2/PDA/PMMA, excitation 482 nm.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXXF
PDA-NH2/PDA/PMMA films with CTAB) exhibits a distinctabsorbance peak at 500 nm.24 The red-orange PDA phase(shown is the UVvis absorbance of the PDA/PMMA or PDA-NH2/PDA/PMMA following incubation with C12mimCl),however, displays the typical absorbance of red-phase PDA ataround 540 nm,23 although the shoulder apparent in a lowerwavelength suggests a contribution from the yellow PDA phase.The purple PDA/PMMA (induced by Triton X-100) gave riseto UVvis spectra that either reflect incomplete blue-redtransformation, or a mixture of the blue and red phases.48
Dramatic differences between the analyte-induced chromatictransformations are apparent in the fluorescence emissionspectra (excitation 482 nm, Figure 5C, D). Surprisingly, thefluorescence spectra show that the yellow PDA film (followingaddition of CTAB) hardly exhibits fluorescence emission,similar to the nonfluorescent blue PDA. This observation, notreported previously, echoes the shifted visible absorbance peakrecorded for the yellow PDA/PMMA films (Figure 5A-B) andindicates that the yellow phase corresponds to a distinct PDAorganization. In a sharp contrast, the red-phase PDA, formedthrough incubation of PDA/PMMA or PDA-NH2/PDA/PMMA with C12mimCl, was highly fluorescent (red curvesin Figure 5C, D), whereas the purple PDA/PMMA films(induced by Triton X-100) produced intermediate emissionspectra. Together, the UVvis and fluorescence emission datain Figure 5 indicate that the dramatic color transitionsrecorded, i.e., blue-purple, blue-red, and blue-yellow (Figures3 and 4), are associated with formation of distinct PDA phases.Moreover, the spectroscopic data in Figure 5 corroborate thecolorimetric analysis above, and confirm that binding ofmolecules from each analyte family resulted in differentstructural/photophysical PDA transformations.
CONCLUSIONSIn conclusion, we present a new PDA film assembly depositedvia noncovalent interactions (i.e., spin-coating) upon trans-parent PMMA substrates. The PDA/PMMA systems exhibitinteresting chromatic properties, likely related to the specificmolecular rearrangement at the PDA/PMMA interface. Indeed,the solvent mixture employed for spin-coating the diacetylenemonomers upon the PMMA substrate (THF/DCM) inducespartial dissolution of the polymer surface area, thereby enablingmore pronounced internalization of the pendant PDA side-chains within the polymer network. Specifically, we observed aunique red-purple transformation induced upon uv irradiationreflecting a reversible transition from the red PDA phase backto the initial blue phase. Furthermore, we detected distinctivecolorimetric and spectroscopic transformations, correspondingto purple, red, and yellow PDA phases specifically induced bydifferent surfactant classes. Overall, this work introduces a newpolymer-supported PDA film construct exhibiting interestingstructural, photophysical, and sensing properties.
AUTHOR INFORMATIONCorresponding Author*E-mail: [email protected] authors declare no competing financial interest.
ACKNOWLEDGMENTSR.J. is grateful to BGNegev Technologies for generous financialsupport. D.M., P.G., and E.T. acknowledge the ministry MiUR
and the University of Bologna (Polo Scientifico Didattico diRavenna, RFO) for funding. We thank Dott. Chiara Samori forthe synthesis of C12LG.
REFERENCES(1) Wegner, G. Topochemical Reactions of Monomers withConjugated Triple Bonds I. Polymerization of 2.4-Hexadiyn-1.6-Diols Derivatives in Crystalline State. Z. Naturoforsch. B 1969, 24,824832.(2) Sun, X.; Chen, T.; Huang, S.; Li, L.; Peng, H. ChromaticPolydiacetylene with Novel Sensitivity. Chem. Soc. Rev. 2010, 39,42444257.(3) Dong, J. A.; Kim, J. M. Fluorogenic Polydiacetylene Supra-molecules: Immobilization, Micropatterning, and Application to Label-Free Chemosensors. Acc. Chem. Res. 2008, 41, 805816.(4) Jelinek, R.; Ritenberg, M. Polydiacetylenes-Recent MolecularAdvances and Applications. RSC Adv. 2013, 3, 2119221201.(5) Yarimaga, O.; Jaworski, J.; Yoon, B.; Kim, J. M. Polydiacetylenes:Supramolecular Smart Materials with a Structural Hierarchy forSensing, Imaging and Display Applications. Chem. Commun. 2012, 48,24692485.(6) Diegelmann, S. R.; Hartman, N.; Markovic, N.; Tovar, J. D.Synthesis and Alignment of Discrete Polydiacetylene-Peptide Nano-structures. J. Am. Chem. Soc. 2012, 134, 20282031.(7) Reppy, M. A.; Pindzola, B. A. Biosensing with PolydiacetyleneMaterials: Structures, Optical Properties and Applications. Chem.Commun. 2007, 42, 43174338.(8) Zou, G.; Jiang, H.; Zhang, Q.; Kohn, H.; Manaka, T.; Iwamoto,M. Chiroptical Switch Based on Azobenzene-Substituted Polydiacety-lene Lb Films under Thermal and Photic Stimuli. J. Mater. Chem.2010, 20, 285291.(9) Lee, J.; Kim, H. J.; Kim, J. Polydiacetylene Liposome Arrays forSelective Potassium Detection. J. Am. Chem. Soc. 2008, 130, 50105011.(10) Park, C. H.; Kim, J. P.; Lee, S. W.; Jeon, N. L.; Yoo, P. J.; Sim, S.J. A Direct, Multiplex Biosensor Platform for Pathogen DetectionBased on Cross-Linked Polydiacetylene (Pda) Supramolecules. Adv.Funct. Mater. 2009, 19, 37033710.(11) Wu, J.; Zawistowski, A.; Ehrmann, M.; Yi, T.; Schmuck, C.Peptide Functionalized Polydiacetylene Liposomes Act as aFluorescent Turn-on Sensor for Bacterial Lipopolysaccharide. J. Am.Chem. Soc. 2011, 133, 97209723.(12) Gravel, E.; Ogier, J.; Arnauld, T.; MacKiewicz, N.; Duconge, F.;Doris, E. Drug Delivery and Imaging with Polydiacetylene Micelles.Chem. - Eur. J. 2012, 18, 400408.(13) MacKiewicz, N.; Gravel, E.; Garofalakis, A.; Ogier, J.; John, J.;Dupont, D. M.; Gombert, K.; Tavitian, B.; Doris, E.; Duconge, F.Tumor-Targeted Polydiacetylene Micelles for in Vivo Imaging andDrug Delivery. Small 2011, 7, 27862792.(14) Wacharasindhu, S.; Montha, S.; Boonyiseng, J . ;Potisatityuenyong, A.; Phollookin, C.; Tumcharern, G.;Sukwattanasinitt, M. Tuning of Thermochromic Properties ofPolydiacetylene toward Universal Temperature Sensing Materialsthrough Amido Hydrogen Bonding. Macromolecules 2010, 43, 716724.(15) Kolusheva, S.; Yossef, R.; Kugel, A.; Katz, M.; Volinsky, R.;Welt, M.; Hadad, U.; Drory, V.; Kliger, M.; Rubin, E.; Porgador, A.;Jelinek, R. Array-Based Disease Diagnostics Using Lipid/Polydiacety-lene Vesicles Encapsulated in a Sol-Gel Matrix. Anal. Chem. 2012, 84,59255931.(16) Xu, Q.; Lee, S.; Cho, Y.; Kim, M. H.; Bouffard, J.; Yoon, J.Polydiacetylene-Based Colorimetric and Fluorescent Chemosensor forthe Detection of Carbon Dioxide. J. Am. Chem. Soc. 2013, 135,1775117754.(17) Wang, X.; Sun, X.; Hu, P. A.; Zhang, J.; Wang, L.; Feng, W.; Lei,S.; Yang, B.; Cao, W. Colorimetric Sensor Based on Self-AssembledPolydiacetylene/Graphene- Stacked Composite Film for Vapor-Phase
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXXG
Volatile Organic Compounds. Adv. Funct. Mater. 2013, 23, 60446050.(18) Yoon, J.; Chae, S. K.; Kim, J. M. Colorimetric Sensors forVolatile Organic Compounds (Vocs) Based on Conjugated Polymer-Embedded Electrospun Fibers. J. Am. Chem. Soc. 2007, 129, 30383039.(19) Choi, H.; Choi, I. S.; Lee, G. S.; Ahn, D. J. Fluorescence SignalEnhancement of Polydiacetylene Vesicle Stacks. J. Nanosci. Nano-technol. 2011, 11, 62036207.(20) Ye, Q.; You, X.; Zou, G.; Yu, X.; Zhang, Q. Morphology,Structure and Chromatic Properties of Azobenzene-SubstitutedPolydiacetylene Supramolelular Assemblies. J. Mater. Chem. 2008,18, 27752780.(21) Chen, X.; Kang, S.; Kim, M. J.; Kim, J.; Kim, Y. S.; Kim, H.; Chi,B.; Kim, S. J.; Lee, J. Y.; Yoon, J. Thin-Film Formation of Imidazolium-Based Conjugated Polydiacetylenes and Their Application for SensingAnionic Surfactants. Angew. Chem., Int. Ed. 2010, 49, 14221425.(22) Dei, S.; Matsumoto, A. Thermochromism of Polydiacetylenes inthe Solid State and in Solution by the Self-Organization of PolymerChains Containing No Polar Group. Macromolecules 2008, 41, 24672473.(23) Lee, S.; Lee, K. M.; Lee, M.; Yoon, J. Polydiacetylenes BearingBoronic Acid Groups as Colorimetric and Fluorescence Sensors forCationic Surfactants. ACS Appl. Mater. Interfaces 2013, 5, 45214526.(24) Lee, J.; Yarimaga, O.; Lee, C. H.; Choi, Y. K.; Kim, J. M.Network Polydiacetylene Films: Preparation, Patterning, and SensorApplications. Adv. Funct. Mater. 2011, 21, 10321039.(25) Carpick, R. W.; Sasaki, D. Y.; Marcus, M. S.; Eriksson, M. A.;Burns, A. R. Polydiacetylene Films: A Review of Recent Investigationsinto Chromogenic Transitions and Nanomechanical Properties. J.Phys.: Condens. Matter. 2004, 16, R679R697.(26) Jiang, H.; Pan, X. J.; Lei, Z. Y.; Zou, G.; Zhang, Q. J.; Wang, K.Y. Control of Supramolecular Chirality for Polydiacetylene Lb Filmswith the Command Azobenzene Derivative Monolayer. J. Mater. Chem.2011, 21, 45184522.(27) Ritenberg, M.; Kolusheva, S.; Ganin, H.; Meijler, M. M.; Jelinek,R. Biofilm Formation on Chromatic Sol-Gel/Polydiacetylene Films.ChemPlusChem. 2012, 77, 752757.(28) You, X.; Zou, G.; Ye, Q.; Zhang, Q.; He, P. Ruthenium(II)Complex-Sensitized Solid-State Polymerization of Diacetylene in theVisible Light Region. J. Mater. Chem. 2008, 18, 47044711.(29) Jiang, H.; Pan, X. J.; Lei, Z. Y.; Zou, G.; Zhang, Q. J.; Wang, K.Y. Photocontrol of Chiroptical Properties of Polydiacetylene CarryingAzobenzene in the Side Chain. Chem. Phys. Lett. 2010, 500, 100103.(30) Tariq, M.; Freire, M. G.; Saramago, B.; Coutinho, J. A. P.;Lopes, J. N. C.; Rebelo, L. P. N. Surface Tension of Ionic Liquids andIonic Liquid Solutions. Chem. Soc. Rev. 2012, 41, 829868.(31) Gal, N.; Malferarri, D.; Kolusheva, S.; Galletti, P.; Tagliavini, E.;Jelinek, R. Membrane Interactions of Ionic Liquids: PossibleDeterminants for Biological Activity and Toxicity. Biochim. Biophys.Acta, Biomembr. 2012, 1818, 29672974.(32) Nockemann, P.; Binnemans, K.; Driesen, K. Purification ofImidazolium Ionic Liquids for Spectroscopic Applications. Chem. Phys.Lett. 2005, 415, 131136.(33) Earle, M. J.; Gordon, C. M.; Plechkova, N. V.; Seddon, K. R.;Welton, T. Decolorization of Ionic Liquids for Spectroscopy. Anal.Chem. 2007, 79, 758764.(34) Paytash, P. L.; Sparrow, E.; Gathe, J. C. The Reaction of ItaconicAcid with Primary Amines. J. Am. Chem. Soc. 1950, 72, 14151416.(35) Galletti, P.; Moretti, F.; Samor, C.; Tagliavini, E. EnzymaticAcylation of Levoglucosan in Acetonitrile and Ionic Liquids. GreenChem. 2007, 9, 987991.(36) Volinsky, R.; Kliger, M.; Sheynis, T.; Kolusheva, S.; Jelinek, R.Glass-Supported Lipid/Polydiacetylene Films for Colour Sensing ofMembrane-Active Compounds. Biosens. Bioelectron. 2007, 22, 32473251.(37) Pevzner, A.; Kolusheva, S.; Orynbayeva, Z.; Jelinek, R. GiantChromatic Lipid/Polydiacetylene Vesicles for Detection and Visual-
ization of Membrane Interactions. Adv. Funct. Mater. 2008, 18, 242247.(38) Giorgetti, E.; Muniz-Miranda, M.; Margheri, G.; Giusti, A.;Sottini, S.; Alloisio, M.; Cuniberti, C.; Dellepiane, G. Uv Polymer-ization of Self-Assembled Monolayers of a Novel Diacetylene onSilver: A Spectroscopic Analysis by Surface Plasmon Resonance andSurface Enhanced Raman Scattering. Langmuir 2006, 22, 11291134.(39) Xu, Y.; Li, J.; Hu, W.; Zou, G.; Zhang, Q. Thermochromism andSupramolecular Chirality of the Coumarin-Substituted PolydiacetyleneLb Films. J. Colloid Interface Sci. 2013, 400, 116122.(40) Cui, C.; Choi, H.; Lee, G. S.; Ahn, D. J. Fluorescence Switch inRed-Phase Polydiacetylene Films and Vesicles Upon Thermal Cycles.J. Nanosci. Nanotechnol. 2011, 11, 57545760.(41) Seo, S.; Lee, J.; Choi, E.-J.; Kim, E.-J.; Song, J.-Y.; Kim, J.Polydiacetylene Liposome Microarray toward Influenza a VirusDetection: Effect of Target Size on Turn-on Signaling. Macromol.Rapid Commun. 2013, 34, 743748.(42) Cho, Y.-S.; Kim, K. M.; Lee, D.; Kim, W. J.; Ahn, K. H. Turn-onFluorescence Detection of Apoptotic Cells Using a Zinc(Ii)-Dipicolyl-amine-Functionalized Poly(Diacetylene) Liposome. Chem.Asian J.2013, 8, 755759.(43) Foley, P.; Kermanshahi Pour, A.; Beach, E. S.; Zimmerman, J. B.Derivation and Synthesis of Renewable Surfactants. Chem. Soc. Rev.2012, 41, 14991518.(44) Franklin, R. In Surfactants from Renewable Resources; Kjellin, M.,Johansson, I., Eds; John Wiley and Sons: West Sussex, U.K., 2010;Chapter 2, pp 2143.(45) Willke, T.; Vorlop, K. D. Industrial Bioconversion of RenewableResources as an Alternative to Conventional Chemistry. Appl.Microbiol. Biotechnol. 2004, 66, 131142.(46) Shafizadeh, F.; Furneaux, R. H.; Cochran, T. G.; Scholl, J. P.;Sakai, Y. Production of Levoglucosan and Glucose from Pyrolysis ofCellulosic Materials. J. Appl. Polym. Sci. 1979, 23, 35253539.(47) Potisatityuenyong, A.; Rojanathanes, R.; Tumcharern, G.;Sukwattanasinitt, M. Electronic Absorption Spectroscopy ProbedSide-Chain Movement in Chromic Transitions of PolydiacetyleneVesicles. Langmuir 2008, 24, 44614463.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am501414z | ACS Appl. Mater. Interfaces XXXX, XXX, XXXXXXH
Click here to load reader